Module 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory. Introduction: The Lecture Contains: Laminate Theory with Thermal Effects


 Ruby Hardy
 1 years ago
 Views:
Transcription
1 Module 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory Introduction: In this lecture we are going to develop the laminate theory with thermal and hygral effects. Then we will develop the relations for effective coefficients of thermal and hygral expansion for laminate. Further, we will develop governing differential equation for laminate. We will conclude this lecture with some sample numerical examples based on this. The Lecture Contains: Laminate Theory with Thermal Effects Laminate Coefficient of Thermal Expansion Laminate Theory with Hygral Effects Laminate Coefficients of Hygral Expansion Hygrothermal Effects on Laminate Governing Differential Equations for Classical Laminate Theory Examples Homework References file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture19/19_1.htm[8/18/ :40:56 PM]
2 Module 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory Laminate Theory with Thermal Effects: In the classical laminate theory we make the assumption that the total strain is superposition of mechanical strain and thermal strains. Thus, (5.96) where, laminate as is the thermal strain in laminate. We can write the stresses in global direction for Thus, using Equation (5.95) in above equation, we get (5.97) Now we find the resultant inplane forces as Recalling the development of classical laminate theory with the use of Equation (5.21), we write (5.98) Let us define (5.99) as the effective laminate thermal forces per unit length. Thus, with this definition we can write Equation (5.97) as (5.100) file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture19/19_2.htm[8/18/ :40:56 PM]
3 Now let us define the resultant moments using Equation (5.96) as With the use of Equation (5.21) and Equation (5.27), we write (5.101) Let us define (5.102) as the effective laminate thermal moments per unit length. Thus, with this definition we can write Equation (5.101) as (5.103) Combining Equation (5.99) and Equation (5.102), we write (5.104) The inverse of this equation is written as (5.105) file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture19/19_2.htm[8/18/ :40:56 PM]
4 Module 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory Laminate Coefficient of Thermal Expansion The derivation of laminate coefficients of thermal expansion is dealt here for symmetric laminates. This is because there is no extensionbending coupling due to the fact that for symmetric laminates. Let us derive the expression for the coefficient of thermal expansion for laminate. Let us define the coefficient of thermal expansion for laminate,, as the laminate midplane strain,, to the per unit uniform change in temperature,. Thus, (5.106) Now for symmetric laminates with pure thermal loading, we have (5.107) Combining Equation (5.105) and Equation (5.106), we get (5.108) For a uniform temperature change the equivalent thermal force is given as (5.109) Thus, the laminate coefficient of thermal expansion becomes (5.110) It is known that the and are constant in each lamina in thickness direction. Thus, the integration over thickness can be simplified as the summation over laminae thicknesses as (5.111) where, is the thickness of kth lamina. Figure 5.12 shows the variation of for laminate along with of layer for for AS4/ Epoxy material from Soden et al [4]. Similarly, Figure 5.13 and Figure 5.14 show the variation of and. From these figures it is seen that these coefficients vary from positive to negative values. Further, it file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture19/19_3.htm[8/18/ :40:57 PM]
5 is observed that the coefficient of thermal expansion depends upon stacking sequence. This fact is very important from laminate designing point of view where it is used in an environment with large thermal gradient. One can choose a laminate sequence for which a coefficient of thermal expansion is zero. From Equation (5.109) and Equation (5.110) for a uniform temperature change, the equivalent thermal force is written as (5.112) Figure 5.12: Variation of for lamina and of for laminate Figure 5.13: Variation of for lamina and of for laminate file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture19/19_3.htm[8/18/ :40:57 PM]
6 Figure 5.14: Variation of for lamina and of for laminate file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture19/19_3.htm[8/18/ :40:57 PM]
7 Module 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory Laminate Theory with Hygral Effects: In this study, the total strain is assumed to be superimposition of mechanical and hygral strains. (5.113) where, is the hygral strain in laminate. The stress in global direction is given as (5.114) The resultant inplane forces are given as (5.115) where, (5.116) is defined as the resultant inplane forces per unit length due to hygral strains. In a similar way, we can give the resultant moments as (5.117) where, (5.118) is defined as resultant moments per unit length due to hygral strains. Combining Equation (5.116) and Equation (5.118), we write (5.119) The inverse of this equation is written as (5.120) file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture19/19_4.htm[8/18/ :40:57 PM]
8 file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture19/19_4.htm[8/18/ :40:57 PM]
9 Module 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory Laminate Coefficients of Hygral Expansion Here we derive the laminate coefficients hygral expansion,, for symmetric laminates. Let us define the coefficient of hygral expansion for laminate as laminate midplane strains to the per percentage change in moisture absorption,. Thus, (5.121) For symmetric laminates with hygral loads alone, we can write (5.122) Combining Equation (5.121) and Equation (5.122), we get (5.123) For a uniform moisture absorption the equivalent hygral force is given as (5.124) Thus, the laminate coefficient of hygral expansion becomes (5.125) It is known that the and are constant in each lamina in thickness direction. Thus, the integration over thickness can be simplified as summation over laminae thicknesses as (5.126) Combining Equation (5.124) and Equation (5.125) we can get the effective hygral force as (5.127) Figure 5.15 shows the variation of for laminate along with of a layer of for T300/5208 material from Pipes et al [5]. Similarly, Figure 5.16 and Figure 5.16 show the variation of and. file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture19/19_5.htm[8/18/ :40:57 PM]
10 Figure 5.15: Variation of for lamina and of for laminate Figure 5.16: Variation of for lamina and of for laminate file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture19/19_5.htm[8/18/ :40:57 PM]
11 Figure 5.17: Variation of for lamina and of for laminate file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture19/19_5.htm[8/18/ :40:57 PM]
12 Module 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory Hygrothermal Effects on Laminate: When thermal as well as hygral strains are present in total strain, then (5.128) The resultant inplane forces are given as (5.129) and the resultant moments are given as (5.130) Equation (5.115) and (5.116) are combined as (5.131) The inverse of this equation is written as (5.132) file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture19/19_6.htm[8/18/ :40:58 PM]
13 Module 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory Governing Differential Equations for Classical Laminate Theory The equilibrium equations for a laminate are (5.133) In the laminate, in general, we consider that the transverse shear stresses are vanishing at the top and bottom of the laminate, that is at and. Now, integrate Equation (5.133) with respect to z. The first two of the above equation give us (5.134) The third of the Equation (5.133) gives (5.135) where, and Now, multiply the first of Equation (5.133) with z and integrate with respect to z to get (5.136) Now, let us write Now recalling that at and we can write for the third term in Equation (5.136) as and file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture19/19_7.htm[8/18/ :40:58 PM]
14 Thus, Equation (5.136) becomes (5.137) Similarly, we can write (5.138) Now putting Equation (5.137) and Equation (5.138) in Equation (5.135) we get (5.139) Note that this equation is identical with the homogeneous plate theory. However, in these equations the definition of the resultants is different. One can express the moment resultants in terms of A, B and D matrices and the derivatives of midplane displacements as given below. Equation (5.137) can be written as (5.140) Equation (5.138) becomes (5.141) And Equation (5.139) becomes (5.142) file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture19/19_7.htm[8/18/ :40:58 PM]
15 Module 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory Examples: Note: In the following examples, each lamina has a thickness of 1 mm and material is AS4/ Epoxy from Soden et al [4]. Example 5.9: For the laminate in Example 5.2 (that is, coefficients of thermal expansions. ), calculate the laminate Solution: This is a symmetric matrix. Hence,. A matrix is given as: Now we have Now we calculate effective thermal forces for fictitious thermal change of. which gives, The laminate coefficients of thermal expansion are calculated as file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture19/19_8.htm[8/18/ :40:59 PM]
16 file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture19/19_8.htm[8/18/ :40:59 PM]
17 Module 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory Example 5.10: For the laminate in Example 5.3 (that is, thermal expansions. ), calculate the laminate coefficients of Solution: This is a symmetric matrix. Hence,. A matrix is given as: And Now we calculate effective thermal forces for fictitious thermal change of. In the thermal force calculation we have assumed that the middle two layers are combined to form one layer of 2 mm thickness. which gives, The laminate coefficients of thermal expansion are calculated as file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture19/19_9.htm[8/18/ :40:59 PM]
18 Example 5.11: Material properties for T300/5208 material are given here [Error! Reference source not found.]. Calculate the laminate coefficients of hygral expansion for laminate with each layer of 1 mm thickness. Solution: This is a symmetric matrix. Hence,. A matrix is given as: And Now we calculate effective thermal forces for fictitious hygral change of. In the hygral force calculation we have assumed that the middle two layers are combined to form one layer of 2 mm thickness file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture19/19_9.htm[8/18/ :40:59 PM]
19 which gives, The laminate coefficients of hygral expansion are calculated as file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture19/19_9.htm[8/18/ :40:59 PM]
20 Module 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory Example 5.12: The laminate in Example 5.1 is subjected to a thermal gradient of. Calculate the thermal residual stress at the top of the laminate. Solution: The matrix for this material is calculated as Now, matrix for and is calculated as The coefficients of thermal expansion in global directions for and layers are and And the A, B and D matrices are calculated as The thermal forces are file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture19/19_10.html[8/18/ :40:59 PM]
21 Now we calculate the thermal moments as We can write for the thermal forces and moments as which becomes, Solving for the midplane strains and curvatures file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture19/19_10.html[8/18/ :40:59 PM]
22 The total strains at the top of the laminate, that is, at in lamina is We calculate the mechanical strains by subtracting the thermal strains from total strains. Now the thermal strain in top lamina is Thus, the mechanical strains become And the stresses at the top of the laminate are given as file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture19/19_10.html[8/18/ :40:59 PM]
23 Module 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory Homework: 1. Derive the resultant inplane forces and moments for a laminate with thermal effects. 2. Derive the resultant inplane forces and moments for a laminate with hygral effects. 3. Derive an expression for laminate coefficient of thermal expansion under the uniform temperature condition. 4. Derive an expression for laminate coefficient of hygral expansion under the condition of uniform moisture absorption. 5. Derive the expressions for resultant inplane forces and moments for a laminate with hygrothermal effects. 6. Derive the governing differential equations for classical laminate theory. 7. Calculate the laminate coefficients of thermal expansion for the following laminates of AS4/ Epoxy from Soden et al [4]. Take thickness of each layer as 1 mm. a. b. c. d. 8. Calculate the thermal residual stresses for a temperature change of at the top and bottom of the following laminates of AS4/ Epoxy. (Write a computer code for this problem. Repeat the Example 5.12). a. b. 9. Calculate the laminate coefficients of hygral expansion for laminate sequences in exercise example 7 with T300/5208 material as in Example Take thickness of each layer as 1 mm. file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture19/19_11.htm[8/18/ :41:00 PM]
24 Module 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory References: CT Herakovich. Mechanics of Fibrous Composites, John Wiley & Sons, Inc. New York, BD Agarwal, LJ Broutman. Analysis and Performance of Fibre Composites, John Wiley & Sons, Inc. New York, AK Kaw. Mechanics of Composite Materials, CRC Press Boca Raton, New York, PD Soden, MJ Hinton, AS Kaddour. Lamina properties, layup configurations and loading conditions for a range of fibrereinforced composite laminates. Composite Science and Technology, 1998;58: RB Pipes, JR Vinson, TW Chou. On the hygrothermal response of laminated composite systems. Journal of Composite Materials, 1976, Vol. 10, pp file:///d /Web%20Course%20(Ganesh%20Rana)/Dr.%20Mohite/CompositeMaterials/lecture19/19_12.htm[8/18/ :41:00 PM]
Module 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationUsing MATLAB to Design and Analyse Composite Laminates
Engineering, 2010, 2, 904916 doi:10.4236/eng.2010.211114 Published Online November 2010 (http://www.scirp.org/journal/eng). Using MATLAB to Design and Analyse Composite Laminates Abstract Avinash Ramsaroop,
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationFinite Element Analysis Prof. Dr. B. N. Rao Department of Civil Engineering Indian Institute of Technology, Madras. Module  01 Lecture  11
Finite Element Analysis Prof. Dr. B. N. Rao Department of Civil Engineering Indian Institute of Technology, Madras Module  01 Lecture  11 Last class, what we did is, we looked at a method called superposition
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More information3D and Planar Constitutive Relations
3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace
More informationFinite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix)
Finite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix) Nikhil J. Chaudhari 1 Post Graduate Student Department of Mechanical Engineering Veermata Jijabai Technological Institute
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationCOMPUTER AIDED DESIGN IN CASE OF THE LAMINATED COMPOSITE MATERIALS
6 th International Conference Computational Mechanics and Virtual Engineering COMEC 15 1516 October 15, Braşov, Romania COMPUER AIDED DESIGN IN CASE OF HE LAMINAED COMPOSIE MAERIALS Camelia Cerbu ransilvania
More informationL e c t u r e. D r. S a s s a n M o h a s s e b
The Scaled smteam@gmx.ch Boundary Finite www.erdbebenschutz.ch Element Method Lecture A L e c t u r e A1 D r. S a s s a n M o h a s s e b V i s i t i n g P r o f e s s o r M. I. T. C a m b r i d g e December
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More information2D damping predictions of fiber composite plates: Layup effects
Available online at www.sciencedirect.com Composites Science and Technology 68 (2008) 727 733 COMPOSITES SCIENCE AND TECHNOLOGY www.elsevier.com/locate/compscitech 2D damping predictions of fiber composite
More informationModule 4 : Deflection of Structures Lecture 4 : Strain Energy Method
Module 4 : Deflection of Structures Lecture 4 : Strain Energy Method Objectives In this course you will learn the following Deflection by strain energy method. Evaluation of strain energy in member under
More informationInternational Journal of Advanced Engineering Technology EISSN
Research Article INTEGRATED FORCE METHOD FOR FIBER REINFORCED COMPOSITE PLATE BENDING PROBLEMS Doiphode G. S., Patodi S. C.* Address for Correspondence Assistant Professor, Applied Mechanics Department,
More informationPresented By: EAS 6939 Aerospace Structural Composites
A Beam Theory for Laminated Composites and Application to Torsion Problems Dr. BhavaniV. Sankar Presented By: Sameer Luthra EAS 6939 Aerospace Structural Composites 1 Introduction Composite beams have
More informationKirchhoff Plates: Field Equations
20 Kirchhoff Plates: Field Equations AFEM Ch 20 Slide 1 Plate Structures A plate is a three dimensional bod characterized b Thinness: one of the plate dimensions, the thickness, is much smaller than the
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 15 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationBasic Energy Principles in Stiffness Analysis
Basic Energy Principles in Stiffness Analysis StressStrain Relations The application of any theory requires knowledge of the physical properties of the material(s) comprising the structure. We are limiting
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationChapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING )
Chapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING ) 5.1 DEFINITION A construction member is subjected to centric (axial) tension or compression if in any cross section the single distinct stress
More informationStructural Analysis III Compatibility of Displacements & Principle of Superposition
Structural Analysis III Compatibility of Displacements & Principle of Superposition 2007/8 Dr. Colin Caprani, Chartered Engineer 1 1. Introduction 1.1 Background In the case of 2dimensional structures
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationCHAPTER 3 THE EFFECTS OF FORCES ON MATERIALS
CHAPTER THE EFFECTS OF FORCES ON MATERIALS EXERCISE 1, Page 50 1. A rectangular bar having a crosssectional area of 80 mm has a tensile force of 0 kn applied to it. Determine the stress in the bar. Stress
More informationLecture 2: Finite Elements
Materials Science & Metallurgy Master of Philosophy, Materials Modelling, Course MP7, Finite Element Analysis, H. K. D. H. Bhadeshia Lecture 2: Finite Elements In finite element analysis, functions of
More informationReview of Strain Energy Methods and Introduction to Stiffness Matrix Methods of Structural Analysis
uke University epartment of Civil and Environmental Engineering CEE 42L. Matrix Structural Analysis Henri P. Gavin Fall, 22 Review of Strain Energy Methods and Introduction to Stiffness Matrix Methods
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationModeling of the Bending Stiffness of a Bimaterial Beam by the Approximation of OneDimensional of Laminated Theory
. FloresDomínguez Int. Journal of Engineering Research and Applications RESEARCH ARTICLE OPEN ACCESS odeling of the Bending Stiffness of a Bimaterial Beam by the Approimation of OneDimensional of Laminated
More informationIntroduction to Continuous Systems. Continuous Systems. Strings, Torsional Rods and Beams.
Outline of Continuous Systems. Introduction to Continuous Systems. Continuous Systems. Strings, Torsional Rods and Beams. Vibrations of Flexible Strings. Torsional Vibration of Rods. BernoulliEuler Beams.
More informationNow we are going to use our free body analysis to look at Beam Bending (W3L1) Problems 17, F2002Q1, F2003Q1c
Now we are going to use our free body analysis to look at Beam Bending (WL1) Problems 17, F00Q1, F00Q1c One of the most useful applications of the free body analysis method is to be able to derive equations
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationAPPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN
28 TH INTERNATIONAL CONGRESS OF THE AERONAUTICAL SCIENCES APPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN Tuyen Tran*, Dan Simkins**, Shen Hin Lim*,
More information*Corresponding author: Keywords: Finiteelement analysis; Multiscale modelling; Onset theory; Dilatational strain invariant.
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MICROMECHANICAL MODELLING OF TEST SPECIMENS FOR ONSET OF DILATATIONAL DAMAGE OF POLYMER MATRIX IN COMPOSITE MATERIALS T. D. Tran 1, D. Kelly 1*, G.
More informationTheory and Practice of Rotor Dynamics Prof. Dr. Rajiv Tiwari Department of Mechanical Engineering Indian Institute of Technology Guwahati
Theory and Practice of Rotor Dynamics Prof. Dr. Rajiv Tiwari Department of Mechanical Engineering Indian Institute of Technology Guwahati Module  2 Simpul Rotors Lecture  2 Jeffcott Rotor Model In the
More informationImplications of failure criteria choices on the rapid concept design of composite grillage structures using multiobjective optimisation
Noname manuscript No. (will be inserted by the editor) Implications of failure criteria choices on the rapid concept design of composite grillage structures using multiobjective optimisation A.J.Sobey
More informationS. Srinivasan, Technip Offshore, Inc., Houston, TX
9 th ASCE Specialty Conerence on Probabilistic Mechanics and Structural Reliability PROBABILISTIC FAILURE PREDICTION OF FILAMENTWOUND GLASSFIBER Abstract REINFORCED COMPOSITE TUBES UNDER BIAXIAL LOADING
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationCombined Stresses and Mohr s Circle. General Case of Combined Stresses. General Case of Combined Stresses con t. Twodimensional stress condition
Combined Stresses and Mohr s Circle Material in this lecture was taken from chapter 4 of General Case of Combined Stresses Twodimensional stress condition General Case of Combined Stresses con t The normal
More informationChapter 12 Plate Bending Elements. Chapter 12 Plate Bending Elements
CIVL 7/8117 Chapter 12  Plate Bending Elements 1/34 Chapter 12 Plate Bending Elements Learning Objectives To introduce basic concepts of plate bending. To derive a common plate bending element stiffness
More informationLecture 3 The Concept of Stress, Generalized Stresses and Equilibrium
Lecture 3 The Concept of Stress, Generalized Stresses and Equilibrium Problem 31: Cauchy s Stress Theorem Cauchy s stress theorem states that in a stress tensor field there is a traction vector t that
More informationPreliminaries: Beam Deflections Virtual Work
Preliminaries: Beam eflections Virtual Work There are several methods available to calculate deformations (displacements and rotations) in beams. They include: Formulating moment equations and then integrating
More information2/23/ WIND PRESSURE FORMULA 2. PERCENT OF ALLOWABLE STRESS 3. FATIGUE DESIGN
Original Title Presented by Northwest Signal copyright 2010 Designing & Building Structural Steel Products since 1976 Primary Users Traffic Signal Strain & Mast Arm Poles Cantilever & Bridge Sign Structures
More informationComposite Materials 261 and 262
Composite Materials 261 and 262 Stefan Hartmann 1 David Moncayo 2 1 DYNAmore GmbH, Stuttgart, Germany 2 Daimler AG, Sindelfingen, Germany 11. LSDYNA Forum 2012, 9.  10. Oktober 2012, Ulm 1 Outline Introduction
More informationComposite Laminate Modeling
omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer WHAT THIS WHITE PAPER
More informationUSER BULLETIN 3: DETERMINATION OF UNSUPPORTED LENGTH RATIO L/Db
USER BULLETIN 3: DETERMINATION OF UNSUPPORTED LENGTH RATIO L/Db The unsupported length ratio (L/Db) is calculated by the automatic Sectional modeler spreadsheet using Dhakal and Maekawa [1]. This method
More informationResidual Force Equations
3 Residual Force Equations NFEM Ch 3 Slide 1 Total Force Residual Equation Vector form r(u,λ) = 0 r = total force residual vector u = state vector with displacement DOF Λ = array of control parameters
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationSemiMembrane and Effective Length Theory of Hybrid Anisotropic Materials
International Journal of Composite Materials 2017, 7(3): 103114 DOI: 10.5923/j.cmaterials.20170703.03 SemiMembrane and Effective Length Theory of Hybrid Anisotropic Materials S. W. Chung 1,*, G. S. Ju
More informationStacking sequences for Extensionally Isotropic, Fully Isotropic and QuasiHomogeneous Orthotropic Laminates.
49th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials 710 April 2008, Schaumburg, IL AIAA 20081940 Stacking sequences for Extensionally Isotropic, Fully Isotropic and QuasiHomogeneous
More informationFlexure: Behavior and Nominal Strength of Beam Sections
4 5000 4000 (increased d ) (increased f (increased A s or f y ) c or b) Flexure: Behavior and Nominal Strength of Beam Sections Moment (kipin.) 3000 2000 1000 0 0 (basic) (A s 0.5A s ) 0.0005 0.001 0.0015
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 4 Pure Bending
EA 3702 echanics & aterials Science (echanics of aterials) Chapter 4 Pure Bending Pure Bending Ch 2 Aial Loading & Parallel Loading: uniform normal stress and shearing stress distribution Ch 3 Torsion:
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationGeneric Strategies to Implement Material Grading in Finite Element Methods for Isotropic and Anisotropic Materials
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Engineering Mechanics Dissertations & Theses Mechanical & Materials Engineering, Department of Winter 1292011 Generic
More informationMECHANICS OF MATERIALS
CHAPTER 6 MECHANCS OF MATERALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf David F. Mazurek Lecture Notes: J. Walt Oler Texas Tech University Shearing Stresses in Beams and Thin Walled Members
More informationBridge deck modelling and design process for bridges
EURussia Regulatory Dialogue Construction Sector Subgroup 1 Bridge deck modelling and design process for bridges Application to a composite twingirder bridge according to Eurocode 4 Laurence Davaine
More informationME 202 STRENGTH OF MATERIALS SPRING 2014 HOMEWORK 4 SOLUTIONS
ÇANKAYA UNIVERSITY MECHANICAL ENGINEERING DEPARTMENT ME 202 STRENGTH OF MATERIALS SPRING 2014 Due Date: 1 ST Lecture Hour of Week 12 (02 May 2014) Quiz Date: 3 rd Lecture Hour of Week 12 (08 May 2014)
More informationCHAPTER 6 BENDING Part 1
Ishik University / Sulaimani Civil Engineering Department Mechanics of Materials CE 211 CHAPTER 6 BENDING Part 11 CHAPTER 6 Bending Outlines of this chapter: 6.1. Chapter Objectives 6.2. Shear and
More informationMicromeso draping modelling of noncrimp fabrics
Micromeso draping modelling of noncrimp fabrics Oleksandr Vorobiov 1, Dr. Th. Bischoff 1, Dr. A. Tulke 1 1 FTA Forschungsgesellschaft für Textiltechnik mbh 1 Introduction Noncrimp fabrics (NCFs) are
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationANALYSIS AND NUMERICAL MODELLING OF CERAMIC PIEZOELECTRIC BEAM BEHAVIOR UNDER THE EFFECT OF EXTERNAL SOLICITATIONS
Third International Conference on Energy, Materials, Applied Energetics and Pollution. ICEMAEP016, October 3031, 016, Constantine,Algeria. ANALYSIS AND NUMERICAL MODELLING OF CERAMIC PIEZOELECTRIC BEAM
More informationMacaulay s method for a Timoshenko beam
Macaulay s method for a Timoshenko beam N. G. Stephen School of Engineering Sciences, Mechanical Engineering, University of Southampton, Highfield, Southampton SO7 BJ, UK Email: ngs@soton.ac.uk Abstract
More informationDTU Space Carbon Fiber Reinforced Plastic and CFRP projects. Niels Christian Jessen Hans Ulrik NørgaardNielsen
DTU Space Carbon Fiber Reinforced Plastic and CFRP projects Niels Christian Jessen Hans Ulrik NørgaardNielsen Why CFRP + Material properties can be designed + High Specific Stiffness Young's module /
More informationStochastic structural dynamic analysis with random damping parameters
Stochastic structural dynamic analysis with random damping parameters K. Sepahvand 1, F. Saati Khosroshahi, C. A. Geweth and S. Marburg Chair of Vibroacoustics of Vehicles and Machines Department of Mechanical
More informationNumerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints
THEORETICAL & APPLIED MECHANICS LETTERS 1, 041005 (2011) Numerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints M. R. Khoshravan,
More informationSUBSURFACE DAMAGE LOCATION AND IDENTIFICATION USING INFRARED TECHNIQUES
SUBSURFACE DAMAGE LOCATION AND IDENTIFICATION USING INFRARED TECHNIQUES T.R. Emery 1, J. M. DulieuBarton 1, P.R. Cunningham 2 1 University of Southampton, School of Engineering Sciences, SO17 1BJ, UK
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationLinear plate bending and laminate theory
Linear plate bending and laminate theor 4M: Design Tools Eindhoven Universit of Technolog Linear plate bending A plate is a bod of which the material is located in a small region around a surface in the
More information7.4 The Elementary Beam Theory
7.4 The Elementary Beam Theory In this section, problems involving long and slender beams are addressed. s with pressure vessels, the geometry of the beam, and the specific type of loading which will be
More informationFinite Element Modelling with Plastic Hinges
01/02/2016 Marco Donà Finite Element Modelling with Plastic Hinges 1 Plastic hinge approach A plastic hinge represents a concentrated postyield behaviour in one or more degrees of freedom. Hinges only
More informationModule 6. Approximate Methods for Indeterminate Structural Analysis. Version 2 CE IIT, Kharagpur
Module 6 Approximate Methods for Indeterminate Structural Analysis Lesson 35 Indeterminate Trusses and Industrial rames Instructional Objectives: After reading this chapter the student will be able to
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More informationFRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING.
FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING. X. J. Gong, F. Hernandez, G. Verchery. ISAT  Institut Supérieur de l Automobile et des Transports, LRMA  Laboratoire de
More informationTESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS
TESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS I. M. Daniel, J. L. Abot, and K. A. Wang Walter P. Murphy Professor, Departments of Civil and Mechanical Engineering, Robert R. McCormick School of Engineering
More informationGerald Allen Cohen, 83, passed away Oct. 1, 2014, at his home in Laguna Beach.
Dr Gerald Allen Cohen (19312014) Ringstiffened shallow conical shell designed with the use of FASOR for NASA s Viking project in the 1970s. (from NASA TN D7853, 1975, by Walter L. Heard, Jr., Melvin
More informationTHE INFLUENCE OF THERMAL ACTIONS AND COMPLEX SUPPORT CONDITIONS ON THE MECHANICAL STATE OF SANDWICH STRUCTURE
Journal of Applied Mathematics and Computational Mechanics 013, 1(4), 131 THE INFLUENCE OF THERMAL ACTIONS AND COMPLEX SUPPORT CONDITIONS ON THE MECHANICAL STATE OF SANDWICH STRUCTURE Jolanta Błaszczuk
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationBeam Bending Stresses and Shear Stress
Beam Bending Stresses and Shear Stress Notation: A = name or area Aweb = area o the web o a wide lange section b = width o a rectangle = total width o material at a horizontal section c = largest distance
More informationNigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37
Nigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37 APPLICATION OF THE REISSNERS PLATE THEORY IN THE DELAMINATION ANALYSIS OF A THREEDIMENSIONAL, TIME DEPENDENT, NONLINEAR, UNIDIRECTIONAL
More informationBuckling of tensionloaded thinwalled composite plates with cutouts
Buckling of tensionloaded thinwalled composite plates with cutouts T. Kremer, H. Schürmann To cite this version: T. Kremer, H. Schürmann. Buckling of tensionloaded thinwalled composite plates with
More informationAN IMPROVED NUMERICAL MODEL FOR CALCULATING SHIP HULL FRAME TRANSVERSAL STRUCTURE
COMPUTATIONAL MECHANICS New Trends and Applications E. Oñate and S. R. Idelsohn (Eds.) CIMNE, Barcelona, Spain 1998 AN IMPROVED NUMERICAL MODEL FOR CALCULATING SHIP HULL FRAME TRANSVERSAL STRUCTURE Oscar
More informationAdvanced Structural Analysis Prof. Devdas Menon Department of Civil Engineering Indian Institute of Technology, Madras
Advanced Structural Analysis Prof. Devdas Menon Department of Civil Engineering Indian Institute of Technology, Madras Module No. # 5.4 Lecture No. # 30 Matrix Analysis of Beams and Grids (Refer Slide
More informationFinite elementbased elastoplastic optimum reinforcement dimensioning of spatial concrete panel structures
Research Collection Report Finite elementbased elastoplastic optimum reinforcement dimensioning of spatial concrete panel structures Author(s): Tabatabai, Seyed Mohammad Reza Publication Date: 1996 Permanent
More informationElements of Polymer Structure and Viscoelasticity. David M. Parks Mechanics and Materials II February 18, 2004
Elements of Polymer Structure and Viscoelasticity David M. Parks Mechanics and Materials II 2.002 February 18, 2004 Outline Elements of polymer structure Linear vs. branched; Vinyl polymers and substitutions
More informationUSING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE
Volume II: Fatigue, Fracture and Ceramic Matrix Composites USING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE A. D. Resnyansky and
More informationMECHANICS OF MATERIALS
CHAPTER MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Teas Tech Universit Transformations of Stress and Strain 006 The McGrawHill Companies,
More informationSimulation of the Influence of Manufacturing Quality on Thermomechanical Stress of Microvias
As originally published in the IPC APEX EXPO Conference Proceedings. Simulation of the Influence of Manufacturing Quality on Thermomechanical Stress of Microvias Yan Ning, Michael H. Azarian, and Michael
More informationA NEW REFINED THEORY OF PLATES WITH TRANSVERSE SHEAR DEFORMATION FOR MODERATELY THICK AND THICK PLATES
A NEW REFINED THEORY OF PLATES WITH TRANSVERSE SHEAR DEFORMATION FOR MODERATELY THICK AND THICK PLATES J.M. MARTÍNEZ VALLE Mechanics Department, EPS; Leonardo da Vinci Building, Rabanales Campus, Cordoba
More informationLecture 27 Introduction to finite elements methods
Fall, 2017 ME 323 Mechanics of Materials Lecture 27 Introduction to finite elements methods Reading assignment: News: Instructor: Prof. Marcial Gonzalez Last modified: 10/24/17 7:02:00 PM Finite element
More informationInstitute of Structural Engineering Page 1. Method of Finite Elements I. Chapter 2. The Direct Stiffness Method. Method of Finite Elements I
Institute of Structural Engineering Page 1 Chapter 2 The Direct Stiffness Method Institute of Structural Engineering Page 2 Direct Stiffness Method (DSM) Computational method for structural analysis Matrix
More informationARC 341 Structural Analysis II. Lecture 10: MM1.3 MM1.13
ARC241 Structural Analysis I Lecture 10: MM1.3 MM1.13 MM1.4) Analysis and Design MM1.5) Axial Loading; Normal Stress MM1.6) Shearing Stress MM1.7) Bearing Stress in Connections MM1.9) Method of Problem
More informationChapter 3 LAMINATED MODEL DERIVATION
17 Chapter 3 LAMINATED MODEL DERIVATION 3.1 Fundamental Poisson Equation The simplest version of the frictionless laminated model was originally introduced in 1961 by Salamon, and more recently explored
More informationDiscontinuous Distributions in Mechanics of Materials
Discontinuous Distributions in Mechanics of Materials J.E. Akin, Rice University 1. Introduction The study of the mechanics of materials continues to change slowly. The student needs to learn about software
More informationVirtual Work and Variational Principles
Virtual Work and Principles Mathematically, the structural analysis problem is a boundary value problem (BVP). Forces, displacements, stresses, and strains are connected and computed within the framework
More informationMATERIAL MECHANICS, SE2126 COMPUTER LAB 4 MICRO MECHANICS. E E v E E E E E v E E + + = m f f. f f
MATRIAL MCHANICS, S226 COMPUTR LAB 4 MICRO MCHANICS 2 2 2 f m f f m T m f m f f m v v + + = + PART A SPHRICAL PARTICL INCLUSION Consider a solid granular material, a so called particle composite, shown
More informationACCURATE FREE VIBRATION ANALYSIS OF POINT SUPPORTED MINDLIN PLATES BY THE SUPERPOSITION METHOD
Journal of Sound and Vibration (1999) 219(2), 265 277 Article No. jsvi.1998.1874, available online at http://www.idealibrary.com.on ACCURATE FREE VIBRATION ANALYSIS OF POINT SUPPORTED MINDLIN PLATES BY
More information